Characteristics of P-channel SOI LDMOS
Transistor with Tapered Field Oxides
Jongdae Kima), Sang-Gi Kim, Tae Moon Roh, Hoon Soo Park, Jin-Gun Koo, and Dae Yong Kim
A new tapered TEOS oxide technique has been devel- I. INTRODUCTION
oped to use field oxide of the power integrated circuits. It
provides better uniformity of less than 3 % and reproduci- The Lateral Double Diffused MOSFET (LDMOSFET) is
bility. On-resistance of P-channel RESURF (REduced considered to be one of the most desirable devices in smart
SURface Field) LDMOS transistors has been optimized power integrated circuit applications at voltage below 300V,
and improved by using a novel simulation and tapered due to its low on state resistance. The LDMOS structure on
TEOS field oxide on the drift region of the devices. With Silicon-On-Insulator (SOI) substrate has been widely used in
the similar breakdown voltage, at Vgs = −5.0 V , the spe- intelligent power applications because of the implementation of
cific on-resistance of the LDMOS with the tapered field low voltage CMOS signal processing circuits in conjunction
oxide is about 31.5 mΩ ⋅ cm2 , while that of the LDMOS with high voltage LDMOS drivers on the same chip. It has also
with the conventional field oxide is about 57 mΩ ⋅ cm2 . been the advantages of process compatible to VLSI process
and is easy to integrate with other process.
For power devices, specific on-resistance (Rsp) and break-
down voltage are critical to device performance. Advances in
process technology have improved transistor’s packing density
and, consequently, transistor’s specific on-resistance. Different
techniques have been used to reduce specific on-resistance
while keeping the breakdown voltage high. Many studies on
the Rsp and breakdown voltage improvement of LDMOSFET
device have been reported −. However, improvements in
specific on-resistance have been limits in conventional design
geometries because of the long drift region. Furthermore, the
breakdown voltage of this lateral structure is highly dependent
on the distance between the end of the gate and drain diffusion,
called the drift length.
In this paper, a novel p-channel LDMOS structure on SOI
substrate with new tapered TEOS field oxides on the drift re-
gion is proposed in order to prevent boron out-diffusion at high
temperature and reduce current path in the drift region, leading
to the improvement of device on resistance. To ensure the high
voltage capability, the REduceed SURface Field (RESURF)
Manuscript received Septemper 1, 1998; revised June 28, 1999.
technique  and field plates  are used. The breakdown, dc
Electronic mail: email@example.com. and transient characteristics of the device are investigated both
22 Jongdae Kim et al. ETRI Journal, Volume 21, Number 3, September 1999
Fig. 1. The cross section of p-channel SOI LDMOSFET with Fig. 2. The cross section of p-channel SOI LDMOSFET with a
LOCOS field oxide. tapered field oxide. The drift length (B) is shorter
compared to that (A) shown in Fig. 1.
theoretically and experimentally. Optimization of the process
parameters involved in the design of the structure is presented.
This tapered oxide technology can also be used on good step
coverage and junction extension −.
Source Gate Drain
II. PROPOSED DEVICE STRUCTURE AND
OPTIMIZATION n-well p-drift Region
A conventional LDMOS structure is shown in Fig. 1. For the
structure of the device, field oxide using a conventional LOC
OS method is added on the drain side and drift region. The Rsp Si Substrate
is increased significantly due to the longer current path (A) un-
Doping Concentration (cm-3)
derneath the field oxide and impurity out-diffusion that occurs
during the growth phase of the thick field oxide at high tem-
perature −. In order to decrease the Rsp, the current path
and the impurity out-diffusion need to be reduced. The
LDMOS structure with a new tapered field oxide (Fig. 2) on Fig. 3. Simulated LDMOS structure with doping of stripe cell lateral
DMOS using DIOS simulator. This structure shows SOI sub-
the drift region is proposed here to improve Rsp by reducing the strate, drift and well region with impurity concentration and
current path (B) and preventing impurity redistribution in the junction depth.
It is important to improve the device performance by opti-
mizing on-resistance for a given area and a breakdown voltage. The optimized results were obtained when the impurity con-
A cost effective and elegant method to utilize such a trade-off centrations of the drift region with the junction depth of 4 ~ 5
between on-resistance and breakdown voltage is to optimize µm, the channel, and the source/drain regions were
the device layout. Both experimental measurements and device 6 × 1015 / cm 3 , 7 × 1016 / cm3 , and 5 × 1019 / cm 3 respectively.
and process simulations can achieve this goal. In the develop- The optimized values of the drift length (A or B), the length of
ment of the p-LDMOS structure, two dimensional DIOS and gate field plate over the drain region (Lfg), and the length of the
DESSIS  simulations were performed for the structures of drain field plate (Lfd) over the drift region were 15, 5, and 5 µm
Figs. 1 and 2 to obtain the electrical characteristics, doping pro- respectively.
file, junction depth, and studies on high-voltage p-LDMOS de- Device simulations were performed using DESSIS based on
vices. We investigated different device structure and design the date from the DIOS. Figure 4 shows the simulated potential
parameters for device optimization. The simulation results are distribution of the LDMOS with the conventional field oxide,
compared with experimental data for two different device lay- while the simulated potential distribution of the LDMOS with
outs, namely, the conventional and the tapered structures. the tapered field oxide is represented in Fig. 5. As observed in
Process simulations were performed using DIOS and the re- these figures, the breakdown voltage for the structure of Fig. 1
sults were incorporated into 2-D structures as shown in Fig. 3. is limited to 296 V, while the breakdown voltage for the
ETRI Journal, Volume 21, Number 3, September 1999 Jongdae Kim et al. 23
Source = 0 V Gate = 0 V Drain = −296 V Gate Drain
Uniform Field Distribution Peak E-field Point (2.2 x 105 V/cm)
Fig. 4. Equipotential lines in off-state of the p-LDMOS with con- Fig. 6. Electric field distribution of the p-LDMOS with conven-
ventional field oxide, Vg = 0 V and Vd = −296 V (spacing tional field oxide (spacing between adjacent lines = 2×104
between adjacent lines = 10 V ) V/cm). The electric field crowds at the junction of the p-
drift and deep n-well inside bulk.
Source = 0 V Gate = 0 V Drain = −285 V Gate
Peak E-field Points (2.2 x 105 V/cm)
Fig. 5. Equipotential lines in off-state of the p-LDMOS with ta- Fig. 7. Electric field distribution of the p-LDMOS with tapered
pered field oxide, Vg = 0 V and Vd = −285 V (spacing field oxide (spacing between adjacent lines = 2×104 V/cm).
between adjacent lines = 10 V ) The critical field region is the silicon surface near the gate
and the junction of the p-drift and deep n-well inside bulk.
structure of Fig. 2 is 285 V. They can clearly be seen that the electrical field is very high inside the bulk. As a result, there is
electrical field is much more uniformly distributed at the drift very high impact generation rate inside the bulk leading to the
region. This means that, when the supplying voltage increases, breakdown of the device, as shown in Fig. 8. In addition to impact
the p-drift region is completely depleted, yielding an optimized ionization inside the bulk, Fig. 9 shows high impact ionization
RES URF condition and generation of a critical electrical field rate near the gate side. This is due to the curvature near the gate
inside bulk. edge, leading to the high electric field and another impact ioni-
The simulated field distributions in the structures of Figs. 1 zation region. The impact ionization region near the gate edge
and 2 are presented in Figs. 6 and 7, respectively. It can be seen causes a decrease in impact ionization rate inside bulk. As a
that for the structure in Fig. 1, the electric field in the silicon result of division of the im pact ionization region into two, the
surface near the drain is reduced because of RESURF principle total impact ionization rate within the device is effectively de-
and the highest electric field is located inside the bulk, as creased, corresponding to the breakdown voltage improvement.
shown in Fig. 6. Therefore, avalanche breakdown occurs inside The current flows along the silicon surface and the inside bulk
the bulk. In the proposed structure shown in Fig. 7, the highest of the conventional and the proposed structures.
electric field ( 2.2 ×105 V / cm ) exists both on the silicon surface The simulated specific on-resistances of the LDMOS device
near the gate edge and inside the bulk. Therefore, the break- with LOCOS field oxide and the tapered filed oxide were ob-
down is only dependent on the impurity concentration in the tained 55 mΩ ⋅ cm 2 and 32 mΩ ⋅ cm 2 at the breakdown voltages
drift region of the structures of Figs. 1 and 2, to both of which of 298 V and 285 V, respectively when the gate voltage of −5 V
RESURF technique was applied. is applied. These values are consistent with the experimental
Figures 8 and 9 plot impact ionization contours in devices ones although the breakdown voltage is lower than that of the
Figs. 1 and 2. Due to the completely resurfed drift region, the experimental one.
24 Jongdae Kim et al. ETRI Journal, Volume 21, Number 3, September 1999
Current Flow Current Flow
Source Gate Drain Source Gate Drain
Impact Ionization Contours
Impact Ionization Contours
Fig. 8. Impact ion distribution and current flow in drift region of Fig. 9. Impact ion distribution and current flow in drift region of
the p-LDMOS with the conventional field oxide. the p-LDMOS with the tapered field oxide.
III. TAPERED OXIDE TECHNIQUE AND
The new tapered TEOS field oxide was made through 200
Å of thermally grown (850 ℃) screen oxide, thick TEOS oxide
(8000 Å) annealed at 850℃ in N2, and thin TEOS oxide (2000
Å) . In the double-layer structure of the thick TEOS/thin
TEOS layer, the upper layer is etched extremely fast in the buff-
ered HF solution, while the etch rate of the lower layer is slow. The
SEM photograph of the tapered field oxide is shown in Fig. 10,
which shows the taper angle of 40°. The taper angle of the TEOS Si -sub.
oxide varies from near 60° to 20° with no steep portion at the top
of the step. The feature sizes of the tapered field oxides have been
measured with the SEM, as shown in Fig. 10. Five different wafers
were provided from different runs and twenty different regions of Fig. 10. SEM picture of the new tapered field oxide. The taper
each wafer (total 100 points) have been observed. The new tech- angle of the field oxide shows 40° whose value can be
nique provides better uniformity of less than 3 % and reproducibil- changed by TEOS oxide thickness and annealing tem-
ity. This technology is very simple and low temperature process,
compared to others −.
It is well known that the thermal oxidation of silicon at high The p-channel LDMOSFETs were fabricated on SOI wafers
temperature causes redistribution of impurities at the silicon-silicon with 2 µm buried oxide and 8 µm p-epi layer using a standard
dioxide interface. An effect of the thermal oxidation on the distri- 1.2 µm twin well CMOS process to apply RESURF principle
bution of impurity, especially boron, in drift region of LDMOS- and enhance compatibility with CMOS process. The standard
FETs performs very important role in making a device optimiza- LOCOS technology or the tapered TEOS oxidation technology
tion. The distribution of boron after field oxidation using conven- was used for the field oxide on the lightly doped RESURF re-
tional LOCOS or the tapered TEOS oxide technique has been re- gion of the device. A p-well, which forms the drift region of
ported . In the previously reported paper, the boron impurity p-LDMOSFET is implemented by using boron with implant
concentration in the drift region of the device prior to field oxida- doses of 2.0 ~ 9.5 × 1012 / cm2 . This implant dose is carefully
tion was 6.7 × 1015 cm −3 . Boron out-diffusion into the field oxide controlled so that the RESURF principle is satisfied. The
is, however, observed from the surface of the drift region with n-well implant dose of 1.0 ~ 4.0 × 1013 / cm2 using phospho-
conventional field oxide, resulting in the concentration of rus at 125 keV is followed for the channel region of the high
4.2 × 1015 cm −3 , while boron out-diffusion into the field oxide is voltage p-LDMOSFET. The n- and p-well are annealed at
very small (~ 6.7 × 1015 cm−3 ) when the tapered TEOS field oxide 1150 °C to obtain 3.0 ~ 4.5 µm junction depth. The gate oxide
is used as a field oxide of the p-LDMOSFETs. of 500 Å and second metal of 1.5 µm were used. The re-
maining process is a standard 1.2 µm analog CMOS process.
ETRI Journal, Volume 21, Number 3, September 1999 Jongdae Kim et al. 25
-500 350 150
Specific On-Resistance (mΩ·cm2)
Specific On-Resistance (mΩ.cm )
RESURF Bulk Breakdown Range
I-V for the conventional LDMOS
I-V for the proposed LDMOS 125
Breakdown Voltage (V)
Breakdown Voltage (V)
Drain Current (µA)
VGS = −5.0 V
Drain Current (µA)
-300 VGS = −4.0 V
V =-4.0 V VGS −5.0
GS VGS ==-5.0 V 250
VGS −4.0 V
VGS = =-4.0V 75
Surface Breakdown Range
0 100 0
-500 0 2 4 6 8 10 12
Drain Voltage (mV)
Drain Voltage (mV) Implant Dose in Drift Region ( (x 1E12 cm-2))
Implant Dose in Drift Region × −2
Fig. 11. Forward on-resistance characteristics of LDMOS devices Fig. 12. The distribution of specific on resistance and breakdown
with the conventional field oxide (dot line) and the tapered voltage as a function of boron dose in drift region. The
TEOS field oxide (solid line). The proposed LDMOSFET filled symbols represent the values obtained from the
has twice drain current compared to the conventional devices with conventional field oxide, while the empty
LDMOSFET. symbols indicate the values obtained from the devices
with tapered field oxide.
IV. EXPERIMENTAL RESULTS AND Experimental results of the Rsp and breakdown voltage as a
DISCUSSION function of boron RESURF implantation into deep n-well are
illustrated in Fig. 12. The characteristics show that Rsp de-
The on state characteristics for the LDMOS devices with the creases with increasing boron doping for a given n-type drift
conventional field oxide and the tapered field oxide are shown region concentration. At low boron doses, the ava- lanche
in Fig. 10. At V gs = − 5 .0 V , based on the current-voltage breakdown occurs at silicon surface near the drain and the gate
characteristics in Fig. 10, calculated specific on-resistance for edge because the highest electric field exists on the silicon sur-
the device with the conventional field oxide is given by face near the drain. As boron dose is increased
( 5 ~ 8 × 1012 cm −2 ) a maximum bulk RESURF breakdown is
Rsp = 110 mV / 59.1 µA ⋅ 3.0 × 10 −5 cm 2 = 57 mΩ ⋅ cm 2 . achieved due to the RESURF principle and the highest electric
field located inside the bulk. At high boron dose ( > 8 ×
The calculated specific on-resistance for the device with the 1012 cm −2 ), the avalanche breakdown also occurs at silicon
tapered field oxide is as follows.
surface near the drain and the gate edge because the highest
electric field exists on the silicon surface near the drain. There-
Rsp = 270 mV / 257.6 µA ⋅ 3.0 × 10 −5 cm 2 = 31.5 mΩ ⋅ cm 2
fore, the avalanche breakdown is only dependent on the impu-
rity concentration in the drift region of the structures of Figs. 1
when the gate voltage of − 5 V is applied. From the experi-
and 2, to both of which RESURF technique was applied. It is
mental results, the specific on-resistance for the proposed
also shown in the figure that with the similar breakdown volt-
structure is improved by 40 % compared to the conventional
structure. The reason is that the TEOS field oxidation at low age, the on- resistance can be improved by 35 % or more with
temperature prevents the out-diffusion at the surface for a given this proposed structure. This is due to the reducing the current
RESURF region and shortens the drift length (B) of the pro- path of 1.5 µm and the preventing the out-diffusion of impurity
posed structure. The final difference between A and B in Figs. 1 from the surface of the drift region.
and 2 is about 1.5 ~ 1.6 µm when the field oxide thickness is The electrical characteristics of Rsp and BVDSS for 100
8500 Å. p-LDMOSFETs supplied by 5 different wafers have been also
A similar breakdown characteristic has been reported by our measured. The uniformity of Rsp and VBDSS are less than 5 %
previous paper . The breakdown voltages of the conven- and 3 %, respectively. The IDSS leakage current is less than 1
tional LDMOS and the proposed LDMOS are limited to 305 V nA in both LOCOS structure and the tapered structure whose
and 295 V, corresponding to only 5 % difference between the value was measured by Tektronix Programmable Curve tracer
conventional one and the proposed one. 370 A at the supplied voltage of −300 V.
26 Jongdae Kim et al. ETRI Journal, Volume 21, Number 3, September 1999
V. CONCLUSION  J. C. North, T. E. McGahan, D. W. Rice, and A. C. Adams, “Ta-
pered Windows in Phosphorus-Doped SiO2 by Ion Implantation,”
A new tapered TEOS oxide technique has been developed to IEEE Trans. Electron Devices, Vol. ED-25, 1978, pp. 809−812.
use field oxide of the power integrated circuits. Reproducible  Y. I. Choi, Y. S. Kwon, and C. K. Kim, “Graded Etching of Thermal
Oxide with Various Angles Using Silica Film,” IEEE EDL, Vol.
tapered field oxide (~1 µm thickness) has been formed in
EDL-1, 1980, pp. 30−31.
TEOS oxide by use of a double-layer structure and low tem-
 K. Suzuki, H. Yamawaki, and Y. Tada, “Boron out Diffusion from
perature annealing process, producing a uniform taper of 20° −
Si Substrates in Various Ambients,” Solid-State Electron., Vol. 41,
60°. This technology is very simple and provides better uni- No. 8, 1997, pp. 1095−1097.
formity of less than 3 % and reproducibility.  T. Kato and Y. Nishi, “Redistribution of Diffused Boron in Silicon
Using process and device simulation, it is shown that the by Thermal Oxidation,” Japan. J. of Appl. Phys., Vol. 3, No. 7,
conventional and the proposed structure of p-LDMOS transis- 1964, pp. 377−383.
tors exploit the RESURF principle that results in reduced sur-  DIOS AND DESSIS User’s Manual, ISE, Jan. 1995.
face electric fields and thus improve the breakdown voltage.  Jongdae Kim, Sang-Gi Kim, Tae Moon Roh, Jin Gun Koo, and
This enables device structure optimization using device simu- Kee-Soo Nam, “A Novel p-channel SOI LDMOS Transistor with
lation, leading to a drastic reduction of on-resistances. Tapered Field Oxides,” Proceeding of ISPSD ’98, 1998, pp.
On-resistance of P-channel RESURF LDMOS transistors 375−378.
has been improved by using the novel tapered TEOS field ox-
ide on the drift region of the devices. With the similar break- Jongdae Kim received the B.S. and M.S. de-
down voltage (5 % reduction), the on-resistance can be im- grees in electronics engineering from Kyung-
proved by 35 % or more with the proposed p-LDMOSFET. pook National University, Taegu, Korea, in
This is due to the reducing of the current path and preventing 1982 and 1984, respectively. In 1994 he re-
out-diffusion of impurity from the lightly doped RESURF re- ceived the Ph.D. degree in electrical and com-
gion. The uniformities of Rsp and VBDSS are less than 5 %and puter engineering from the University of New
3 %, respectively. The IDSS leakage current of the LDMOS Mexico in USA. From 1984 to 1989, he was
with the tapered field oxide is less than nA at the supplied volt- with the Electronics and Telecommunications
Research Institute (ETRI), Taejon, Korea, where he worked on silicon
age of −300 V.
based device design and process integration of EEPROM and CMOS.
In 1994 he joined the ETRI and is currently engaged in research on
REFERENCES power integrated circuits for FED and PDP driving ICs. He has pub-
lished over 40 technical papers throughout the major journals and con-
 P. G. Y. Tsui, P. V. Gilbert, and S. W. Sun, “Integration of Power ferences.
LDMOS into a Low-Voltage 0.5 µm BiCMOS Technology,”
IEEE IEDM Digest, 1992, pp. 27−30. Sang-Gi Kim received the M.S. and Ph.D. de-
 L. Vestling, B. Edhholm, J. Olsson, S. Tiensuu, and A. Soderbrag, grees, all in department of physics from Yeung-
“A Novel High-Frequency LDMOS Transistor Using an Ex- nam University, Taegu, Korea, in 1989 and
tended Gate RESURF Technology,” Proceeding of ISPSD ’97, 1996, respectively. In 1981, he joined Semi-
1997, pp. 45−48. conductor Division of Electronics and
 K. Kobayashi, Y. Ninomiya, M. Takahashi, and M. Maruoka, Telecommunications Research Institute, Taejon,
“Development of Process for Low On-Resistance Vertical Power Korea, where he has been working on materials
MOSFETs,” NEC Res. & Develop., Vol. 35, No. 4, 1994, pp. science and device characterization in advanced
433−437. power device technologies. His work also includes novel process
 Jongdae Kim, Mun-Yang Park, Jin Yeong Kang, Sangyong Lee, technologies related to dry etching and CMP process.
Jin-Gun Koo, and Kee-Soo Nam, “Integration of 5-V CMOS and
High-Voltage Devices for Display Driver Applications,” ETRI Tae Moon Roh received the B. S., M. S. and Ph.
Journal, Vol. 20, No. 1, 1998, pp. 37−46. D. degrees in electronic engineering from Kyung-
. J. A. Appels and H. M. J. Vaes, “High Voltage Thin Layer Devices pook National University, Taegu, Korea, in 1984,
(RESURF Devices),” IEEE IEDM Digest, 1979, pp. 238−241. 1986 and 1998, respectively. His doctoral re-
 S. K. Ghandhi, Semiconductor Power Devices, Wiley, New York, search involved the reliability of ultrathin oxide
1997. grown by high pressure oxidation and followed
 H. S. Kim, S. D. Kim, M. K. Han, S. N. Yoon, and Y. I. Choi, by rapid thermal nitridation and hot carrier ef-
“Breakdown Voltage Enhancement of the p-n Junction by fects of MOSFET with those oxide as the gate
Self-Aligned Double Diffusion Process through a Tapered SiO2 insulator. In 1988, he joined Electronics and Telecommunication Re-
Implant Mask,” IEEE EDL, Vol. EDL-16, 1995, pp. 405−407. search Institute, Taejon, Korea. Since 1988, he has worked at
ETRI Journal, Volume 21, Number 3, September 1999 Jongdae Kim et al. 27
ETRI-Micro-Electronics Technology Laboratory, where he has been Jin-Gun Koo was born in Masan, Korea, in
engaged in the research of developing process technology for digital 1955. He received the B.S. and M.E. degrees in
and analog CMOS IC, improving reliability of ultra-thin gate oxide, electronic engineering from Kyungpook Na-
and evaluating hot carrier effects of MOSFETs. His current interests tional University in 1980 and 1992, respectively.
are process technology and reliability of the ultra-thin gate oxide and Form 1980 to 1985, he was with Korean Insti-
MOSFETs. In addition, he works for the development of high voltage tute of Electronics Technology (KIET), where
power IC for flat panel displays and automobiles and BCD technology. he worked on silicon based device design and
process integration of high speed bipolar tran-
Hoon Soo Park received the B.S. degree in sistor. Since 1986, he has been with the Semiconductor fields of Elec-
electronics engineering from Kyungbook Na- tronics and Telecommunications Research Institute (ETRI), where he is
tional University in 1982. He also received M.S., now a head of power device team. His interests involve ASIC, power
and Ph.D. degrees in electronics engineering from IC and semiconductor’s equipment and facility.
Yonsei University, in 1984, and 1991, respectively.
His Ph.D. research focused on development of Dae Yong Kim received the B.S. degree in
CMOS-compatible Smart Power IC. From 1984 electronic engineering from Seoul National
to 1986, he worked as a device engineer at Gold University, Korea in 1974. He received the M.S.
Star Semiconductor Co., where he has been involved in development of and Ph.D. degree in electrical & computer en-
low-power Schottky TTL. From 1993 to 1997, he joined Hyundai gineering from The University of Texas at Aus-
Electronics, System IC Research Center, where he was participated in tin, Texas, USA, in 1985 and 1988, respectively.
development of CMOS and smart power IC technologies as a principal He joined ETRI in 1974, where he is currently
researcher. Since 1997, he has been an assistant professor at Uiduk working as director of
University in Korea. Currently, his research activities are focused on the Semiconductor Processing Department, Micro-Electronics Tech-
development of smart power IC technology, especially in BCD (Bipo- nology Laboratory. His research interests include ASIC technology, RF
lar-DMOS-CMOS) technology. and power IC development.
28 Jongdae Kim et al. ETRI Journal, Volume 21, Number 3, September 1999